advertisement

JOURNAL OF APPLIED PHYSICS 113, 023503 (2013) Anomalous phonon behavior of carbon nanotubes: First-order influence of external load Amin Aghaei,1,a) Kaushik Dayal,1,b) and Ryan S. Elliott2,c) 1 Carnegie Mellon University, Pittsburgh, Pennsylvania 15213, USA Department of Aerospace Engineering and Mechanics, The University of Minnesota, Minneapolis, Minnesota 55455, USA 2 (Received 2 October 2012; accepted 6 December 2012; published online 9 January 2013) External loads typically have an indirect inﬂuence on phonon curves, i.e., they inﬂuence the phonon curves by changing the state about which linearization is performed. In this paper, we show that in nanotubes, the axial load has a direct ﬁrst-order inﬂuence on the long-wavelength behavior of the transverse acoustic (TA) mode. In particular, when the tube is force-free, the TA mode frequencies vary quadratically with wave number and have curvature (second derivative) proportional to the square-root of the nanotube’s bending stiffness. When the tube has non-zero external force, the TA mode frequencies vary linearly with wave number and have slope proportional to the square-root of the axial force. Therefore, the TA phonon curves—and associated transport properties—are not material properties but rather can be directly tuned by external loads. In addition, we show that the out-of-plane shear deformation does not contribute to this mode and the unusual properties of the TA mode are exclusively due to bending. Our calculations consist of 3 parts: First, we use a linear chain of atoms as an illustrative example that can be solved in close-form; second, we use our recently developed symmetry-adapted phonon analysis method to present direct numerical evidence; and ﬁnally, we present a simple mechanical model that captures the essential physics of the geometric nonlinearity in slender nanotubes that couples the axial load directly to the phonon curves. We also compute the density of states and C 2013 American Institute of Physics. show the signiﬁcant effect of the external load. V [http://dx.doi.org/10.1063/1.4774077] I. INTRODUCTION The low-dimensionality of nanotubes causes unusual features in the phonon curves due to geometric effects. In this paper, we examine particularly the transverse acoustic (TA) phonon mode and its slope and curvature (second derivative) in the long wavelength limit. Previous works have reported four acoustic modes of vibration for SWNT. There is consensus that two of the modes (longitudinal and twisting modes) have linear dispersion in the long wavelength limit. However, there has been discussion about the form of the other two TA modes which are doubly degenerate. For example, several papers1–9 report linear dispersion for the TA modes. These authors do not analytically show that the TA modes should be linear, but argue that nanotubes do not have modes analogous to the out-of-plane “bending” mode of graphene, and thus, nanotubes must have linear long wavelength acoustic dispersion behavior. Among these works, two recent papers7,9 state that quadratic dependence is found in some other papers, but argue that this may be attributed to numerical errors. In contrast, more recent papers10–17 report a quadratic dependence of frequency on the wave number. The results presented in these papers are obtained by applying lattice a) Email: aghaei@cmu.edu. Email: kaushik@cmu.edu. c) Email: elliott@aem.umn.edu. b) 0021-8979/2013/113(2)/023503/7/$30.00 dynamics methods to either tight-binding, ab-initio or empirical potential models. In still other papers,18–21 analytical methods are used to argue that the TA mode should be quadratic. In particular, the papers18–20 make an analogy between the phonon dispersion relation and the bending energy or sound velocity in a continuous thin tube. The paper21 develops a spring model and performs lengthy calculations for zig-zag and armchair nanotubes.37 Among these papers, the works11,13,16,18–20 also mention that others have observed linear dependence of the TA dispersion relations. However, these papers do not provide a reason for the discrepancy but rather only postulate that the use of unsuitable force constant parameters may lead to linear TA phonon dispersion. In this paper, we examine the question of the TA phonon dispersion through a combination of explicit calculations in model systems as well as numerical calculations. Our model system consists of a linear chain of atoms as an illustrative example that can be solved in close-form. The numerical calculations are based on recently developed symmetry-adapted methods for nanotubes that allow the examination of bending modes.22,23 Our calculations show that in nanotubes, the axial load has a direct ﬁrst-order inﬂuence on the longwavelength behavior of the TA mode. In particular, when the nanotube is force-free the TA mode frequencies vary quadratically with wave number and have curvature (second derivative) proportional to the square-root of the nanotube’s bending stiffness. When the nanotube has non-zero external force, the TA mode frequencies vary linearly with wave 113, 023503-1 C 2013 American Institute of Physics V Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-2 Aghaei, Dayal, and Elliott J. Appl. Phys. 113, 023503 (2013) number and have slope proportional to the square-root of the axial force. In addition, we show that the out-of-plane shear deformation does not contribute to this mode and the unusual properties of the TA mode are exclusively due to bending. Therefore, the TA phonon curves—and associated transport properties—are not material properties but rather can be directly tuned by external loads. We illustrate this by showing the effect of the external axial load on the density of states (DOS). We develop a simple mechanical model based on classical beam theory that captures the essential physics of the geometric nonlinearity in slender nanotubes that couple the axial load directly to the phonon curves. The paper is organized as follows. We ﬁrst describe what is known in layered nanostructures in Sec. II. We then present the closed-form calculations for atomic chains in Sec. III. In Sec. IV, we present the results of numerical calculations for carbon nanotubes. Finally, in Sec. V, we show that a simple model based on classical beam theory captures the key nonlinearity that governs the TA mode behavior. II. LAYERED CRYSTALS AND ATOMIC SHEET STRUCTURES Transverse in-plane mode: Longitudinal in-plane mode: C11 À C12 2 C44 2 ðkx þ ky2 Þ þ k ; ¼ 2q q z (1) x22 ¼ C11 2 C44 2 ðkx þ ky2 Þ þ k ; q q z (2) Out-of-plane ðbendingÞ mode: C44 2 C33 2 ðk þ ky2 Þ þ k þ K2 ðkx2 þ ky2 Þ2 : x23 ¼ q x q z (4) where r is a measure of the stress in the layer. Thus, the TA bending mode dispersion relation of a stressed layer has a linear dependence on the long wavelength wave vector and has a slope proportional to the square-root of the stress. Making an analogy between layered crystals or sheets and nanotubes, one would then expect similar behavior of the TA phonon modes in nanotubes. In fact, this is exactly what we ﬁnd in Sec. IV from our numerical calculations. III. PHONONS IN A LINEAR ATOMIC CHAIN In this section, we examine a linear atomic chain as a model system that permits closed-form calculations. We show that the TA modes of a linear chain of atoms have linear dependence on the wave number when the chain is subjected to a non-zero axial force. Further, we show that the TA long wavelength phonon modes for a force-free chain correspond to bending, not shear. A. Transverse acoustic phonon modes Quadratic dependence on the wave vector for long wavelength TA phonons is well known in the context of layered crystals, such as graphite, and sheet structures, such as graphene. The ﬁrst works in this area were by Komatsu24,25 (1951) and Lifshitz26 (1952). Their work showed that the TA phonon mode, with wave vector parallel to the layers, is a “bending mode” and has quadratic dispersion. Other works concerned with bending modes in layered crystals include.27–31 The dispersion relation results of these early investigations are summarized in the paper28 as38 x21 r x23 ¼ ðkx2 þ ky2 Þ; q (3) Here, C11 ; C12 ; C33 , and C44 are the elastic constants of the crystal, q is the density, kx and ky are the components of the wave vector parallel to the layer planes, and kz is the component of the wave vector perpendicular to the layers. The quantity K characterizes the bending rigidity of layers and is determined mainly by intralayer forces. For layered crystals, the interlayer elastic constants C33 and C44 are usually negligible compared to K. This illustrates that the predominant contribution to the bending mode dispersion relation is due to the bending rigidity K. It is important to note that Eq. (3) holds for stress-free layers only. If the layer or sheet is subjected to non-zero inplane stress then, according to Lifshitz, the dispersion of the bending mode is For simplicity, we consider a linear chain of atoms which is free to deform in a two-dimensional space. In the conﬁguration of interest, the position vector of atom j is xj ¼ xaj ea ¼ aje1 , where a is the lattice spacing of the chain, e1 is the axial direction of the chain, and a 2 f1; 2g. A standard argument leads to the eigenvalue equation for the phonon frequencies Dk vk ¼ mx2k vk ; (5) where m is the mass of each atom in the chain, k is the wave number (along the axial direction), xk is the phonon frequency, vk is the phonon polarization vector (eigenvector), and Dk is the dynamical matrix given by X H0j exp½Àikx1j : (6) Dk ¼ j Here, Hpq is the Hessian of the chain’s potential energy function / ¼ /ðfxj gÞ. That is, Hpq ¼ @ 2 /=@xp @xq . Due to the Euclidean invariance (objectivity) of the potential energy, we pq gÞ to be a can—without loss of generality—take / ¼ /ðfr function of the pair-distances (rpq k xq À xp k) between atoms in the chain.32 Then, we ﬁnd H0q ¼ ¼ @ 2 r0i @r0i @rqj X @ / X X @2/ þ @r0i @rqj @x0 @xq i6¼0 @r0i @x0 @xq i6¼0 j6¼q X X @2/ 1 ðxi À x0 Þ ðxj À xq Þ @r rqj r @r 0i qj 0i i6¼0 j6¼q þd0q 1 X @/ ½r2 I À ðxi À x0 Þ ðxi À x0 Þ 3 0i @r r 0i 0i i6¼0 Àð1 À d0q Þ 1 @/ 2 ½r0q I À ðxq À x0 Þ ðxq À x0 Þ: (7) 3 @r0q r0q In the standard basis, this becomes Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-3 Aghaei, Dayal, and Elliott ½H0q ab J. Appl. Phys. 113, 023503 (2013) 2XX 6 6 ¼6 6 4 i6¼0 j6¼q i jÀq @2/ @r0i @rqj jij jj À qj 0 From this form of the Hessian, it is clear that the polarization vector for the TA phonon modes of the linear atomic chain is vTA ¼ ½0; 1T . Thus, for this case, the TA dispersion relation is found to be x2TA;k 7 7 7: 1 1 7 X @/ @/ 5 d0q À ð1 À d0q Þ @r jija @r jqja 0i 0q i6¼0 (8) where F is the virial axial force. As can be seen, the change in energy due to shear deformation is not related to the second term of Eq. (11). C. Energy change corresponding to bending deformation 1 X 22 ¼ H0j exp½Àikja m j 1 1 X @/ ð1 À exp½ÀikjaÞ: ¼ m j6¼0 @r0j jjja 3 0 (9) Expanding the exponential in powers of (the small parame ter) k and noting that @ /=@r 0j ¼ @ /=@r0Àj , results in " # " # 3 X À1 @ / 1 X @/ 2 2 3 xTA;k ¼ jjja k þ jjj a k4 þ … 2m j6¼0 @r0j 24m @r 0j j6¼0 (10) Noting that jjja ¼ r0j and neglecting higher order terms, we ﬁnd " # " # 1 X @/ À1 X @ / 2 2 3 r0j k þ r k4 : (11) xTA;k ¼ 2m j6¼0 @r0j 24m j6¼0 @r0j 0j Now consider the chain subjected to bending. The atom with initial position xj ¼ jae1 will move to yj ¼ r½sinðaj=rÞe1 þ cosðaj=rÞe2 , where r is the radius of curvature. The arc length does not change during the bending. If rjl ¼ ðj À lÞa is the separation between atoms j and l before the bending, after bending the separation will be rjl þ Drjl ¼ ½ðy1l À y1j Þ2 þ ðy2l À y2j Þ2 1=2 " 2 2 #1=2 al aj al aj ¼ r 2 cos À cos þ r 2 sin À sin r r r r ! pﬃﬃﬃ al aj al aj 1=2 ¼ 2r 1 À cos cos À sin sin r r r r !1=2 pﬃﬃﬃ rjl aðl À jÞ ¼ 2r 1 À cos ¼ 2r sin 2r r rjl3 : 24r 2 The virial axial force in a chain ofPatoms at zero temperature P @/ P @/ 1 1 can be shown33,34 to be F ¼ 2L i j @rij rij ¼ 2a j @r0j r0j . Thus, the linear part of the dispersion relation (x versus k) is proportional to the square-root of the axial force in the chain. Next, we show that the second term in Eq. (11) is related to the bending stiffness of the chain. This shows that B. Energy change corresponding to shear deformation Expanding the potential energy density up to the ﬁrst order in perturbation gives an energy change of the form If c is the shear parameter in the inﬁnite chain, the displacement of the atoms is u1j ¼ 0 and u2j ¼ cx1j . The separation between the atoms in the deformed chain will be rjl þ Drjl ¼ ½rjl2 þ ðu2l À u2j Þ2 1=2 ¼ ½rjl2 þ c2 rjl2 1=2 ¼ rjl ½1 þ c2 1=2 ! c2 Àc4 þ Á Á Á : (12) % rjl 1 þ þ 2 4 Therefore, the 2 change in distance between the atoms is 2 Drjl % c2 rjl ¼ c2 r0ðjÀlÞ . Expanding the potential energy den~ ¼ /=2N sity, / a, up to the ﬁrst order in perturbation, gives an energy change of the form ~ % D/ ¼ 1 X @/ c2 X @ / Drjl ¼ r0ðjÀlÞ 4Na j;l6¼j @r0ðlÀjÞ 2N a j;l6¼j @rjl c2 X @ / r0n ¼ Fc2 ; 2a n6¼0 @r0n (13) % rjl À (14) Drjl % À ~ ¼ D/ ¼ rjl3 24r 2 : (15) 1 X @/ À1 X @ / Drjl ¼ r3 2Na j;l6¼j @rjl 48Nr 2 a j;l6¼j @r0ðlÀjÞ 0ðjÀlÞ À1 X @ / r3 : 2 24r a n6¼0 @r0n 0n (16) ~ % K 12 ¼ Kj2 , where Hence, we ﬁnd D/ r K¼ À1 X @ / r3 24a n6¼0 @r0n 0n (17) is the bending stiffness and j ¼ 1=r is the bending curvature. Thus, we have shown that the second term on the right hand side of Eq. (11) is related to the bending stiffness K. Consequently, the curvature of the force-free chain’s TA dispersion relation is proportional to the square-root of its bending stiffness. Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-4 Aghaei, Dayal, and Elliott FIG. 1. The distorted shape, i.e., the eigenmode, of the nanotube due to the transverse acoustic mode, near the long-wavelength limit of a (7, 6) nanotube. IV. NUMERICAL CALCULATIONS FOR CARBON NANOTUBES In this section, we use our recently developed symmetryadapted phonon analysis method23 to numerically demonstrate the connection between the TA dispersion relation and the axial force and bending stiffness of a SWNT. The distorted shape, i.e., the eigenmode, of the nanotube due to the transverse acoustic mode, near the long-wavelength limit of a (7, 6) nanotube is plotted in Figure 1. All calculations are performed using the Tersoff interatomic potential.35 Before we describe our results, we note that the paper36 shows, numerically, that bending modes with quadratic dispersion exist in quantum wires with rectangular cross section. The existence of only one continuous wave vector makes the wires similar to nanotubes. However, contrary to nanotubes, because of the rectangular cross section, the bending modes are no longer degenerate in wires. Our systematic symmetry-adapted phonon analysis method is able to deal with the degenerate behavior that occurs in nanotubes and clearly illustrates the quadratic dispersion of the TA phonon modes for a force-free tube. First, we investigate the effect of axial relaxation on the DOS and the form of the dispersion relation for the bending modes. Then, we numerically show that the slope and curvature of the TA modes correspond to the axial force and bending rigidity, respectively. Following the procedures outlined in our previous paper,23 the dispersion curves and DOS for a relaxed J. Appl. Phys. 113, 023503 (2013) (force-free) (7, 6) SWNT are plotted in Fig. 2. Adding axial force leads to one signiﬁcant change of the dispersion curves and DOS. That is, the dispersion of low frequency TA modes changes from quadratic to linear in the long wavelength limit (as k ! h), where h ¼ 0:307p is the rotation angle of the (7, 6) nanotube screw generator. A consequence of the low frequency dispersion curve near k ¼ h is that the DOS is singular near x ¼ 0 for the force-free tube, while conversely, it is almost constant for tubes with non-zero force. This effect is illustrated in Fig. 3, by plotting the long wavelength TA phonon dispersion relation near k ¼ h for tubes subjected to four different values of axial stress. Here, we deﬁne the axial stress as the axial force divided by the force-free circumference of the tube. The ﬁgure shows clear evidence that the long wavelength TA phonon dispersion behavior is related to the axial stress in the SWNT. To show more conclusively that the slope and curvature of the long wavelength TA modes have the speciﬁc dependence postulated in this paper, we compute (1) the bending modulus of SWNTs as a function of tube diameter, (2) the slope of the long wavelength TA phonon mode dispersion relation as a function of axial stress and tube diameter, and (3) the curvature of the long wavelength TA phonon mode dispersion relations for a force-free SWNT as a function tube diameter. We compute the energy density versus curvature relation using zero-temperature objective molecular dynamics (based on Ref. 22 which allows for the explicit control of curvature through a “bending group parameter”) for armchair nanotubes with different diameters. In particular, we ~ ¼ D/=ð‘PÞ, calculate the change in energy density, D/ where ‘ is the objective cell length and P is the perimeter of the nanotube. For each radius, we calculate the bending stiffness K according to ~ ¼ 1 Kj2 D/ 2 ) K¼ ~ 2D/ : 2 j (18) FIG. 2. (Left) Dispersion curves and (right) DOS of zero-force axially relaxed (7, 6) SWNT as described within the symmetry-adapted objective structures framework of paper.23 Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-5 Aghaei, Dayal, and Elliott J. Appl. Phys. 113, 023503 (2013) FIG. 3. The effect of axial stress on (left) the dispersion relation of the TA phonon modes and (right) the DOS of a (7, 6) SWNT. pﬃﬃﬃﬃ Figure 4 shows the variation of K versus the diameter. It is clear that the bending stiffness scales linearly with the square of the diameter. Next, Fig. 5(a) shows the (signed) square of the TA modes’ slope (near k ¼ h) as a function of axial stress for a variety of tube SWNT types. This slope was computed from our phonon dispersion calculations using a numerical differentiation algorithm. Finally, in Fig. 5(b), we show the curvature, computed in a similar manner to the slope, for various nanotubes ranging from (6, 6) to (16, 16) as a function of the tube diameter. From these ﬁgures, we can infer the following important results: • • Fig. 5(a) shows that the slope of the TA mode curve does not depend on the speciﬁc nanotube. It is linearly related to the square root of the axial force. For various nanotubes of different diameters and chiralities, Fig. 5(b) shows that the curvature of the TA mode curve scales linearly with the tube diameter, and Fig. 4 in turn shows that square root of the bending stiffness scales linearly with the tube diameter. Together, these imply that the curvature of the TA mode curve is directly related to the square root of the bending stiffness. These plots, therefore, conﬁrm our claim. V. SIMPLE CONTINUUM MODEL AND DISCUSSION First, we consider the case of a rod that undergoes stretching deformations, but with a pre-stress. This gives us the expected conclusion that the pre-stress plays a role only in determining the equilibrium state around which linearization is conducted. Consider a rod of length L that is extend by an amount d and with a pre-stress r0 . The energy of deformation is, to second order, given by 2 d 1 d þ… E $ r0 þ ET L 2 L Here, ET is the extensional modulus at the state of linearization. The natural frequencies from a normal mode analysis will be proportional to the square root of the coefﬁcient of 1 the quadratic term, i.e., E2T . Now, to understand the current setting, we examine a beam that undergoes transverse deﬂections. Consider a beam of length L, and impose a bending deformation that causes a relative deﬂection D between the ends of the beam. A simple accounting of the geometric nonlinearity shows that there is À Á2 12 À 1 which is simply an extensional strain of 1 þ DL À Á 2 1 D to leading order. The energy of deformation is, to sec2 L ond order, given by 2 1 D þ… E $ r0 2 L FIG. 4. The square root of bending stiffness (calculated by minimizing the energy of armchair nanotubes) versus the diameter of the nanotube. The points are from calculations and the line is a best-ﬁt to the points. (19) (20) The natural frequencies from a normal mode analysis will be proportional to the1 square root of the coefﬁcient of the quadratic term, i.e., r20 . When this term is absent, higher-order effects such as bending control the curvature of the TA mode curve. Therefore, this gives the unusual direct dependence of the normal mode frequencies on the axial force. As the above simple analysis shows, the key to this feature is the geometric nonlinearity of a slender structure. As our calculations above have shown, the density of states can also be tuned signiﬁcantly by applying an axial force. Therefore, it is possible that properties such as heat transfer can be tuned by mechanical means. Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-6 Aghaei, Dayal, and Elliott J. Appl. Phys. 113, 023503 (2013) FIG. 5. (a) Square of the slope of the TA mode vs. the axial stress. (b) Curvature of the TA mode vs. diameter for various nanotubes ranging from (6, 6) to (16, 16). The points are from calculations and the line is a best-ﬁt to the points. ACKNOWLEDGMENTS Amin Aghaei and Kaushik Dayal thank AFOSR Computational Mathematics (FA9550-09-1-0393) and AFOSR Young Investigator Program (FA9550-12-1-0350) for ﬁnancial support. Ryan Elliott acknowledges support from the NSF CAREER Grant No. CMMI-0746628 and The University of Minnesota Supercomputing Institute. Kaushik Dayal also acknowledges support from NSF Dynamical Systems (0926579), NSF Mechanics of Materials (CAREER1150002), and ARO Solid Mechanics (W911NF-10-1-0140). Amin Aghaei also acknowledges support from the Dowd Graduate Fellowship. This work was also supported in part by the NSF through TeraGrid resources provided by Pittsburgh Supercomputing Center. Kaushik Dayal thanks the Hausdorff Research Institute for Mathematics at the University of Bonn for hospitality. We thank Richard D. James for useful discussions. 1 J. Yu, R. K. Kalia, and P. Vashishta, “Phonons in graphitic tubules: A tightbinding molecular dynamics study,” J. Chem. Phys. 103, 6697 (1995). 2 R. Saito, T. Takeya, T. Kimura, G. Dresselhaus, and M. S. Dresselhaus, “Raman intensity of single-wall carbon nanotubes,” Phys. Rev. B 57, 4145 (1998). 3 M. S. Dresselhaus and P. C. Eklund, “Phonons in carbon nanotubes,” Adv. Phys. 49, 705–814 (2000). 4 J. Hone, B. Batlogg, Z. Benes, A. T. Johnson, and J. E. Fischer, “Quantized phonon spectrum of single-wall carbon nanotubes,” Science 289, 1730–1733 (2000). 5 J. Hone, “Phonons and thermal properties of carbon nanotubes,” Top. Appl. Phys. 80, 273–286 (2001). 6 J. Maultzsch, S. Reich, C. Thomsen, E. Dobardzic, I. Milosevic, and M. Damnjanovic, “Phonon dispersion of carbon nanotubes,” Solid State Commun. 121, 471–474 (2002). 7 D. Sanchez-Portal and E. Hernandez, “Vibrational properties of singlewall nanotubes and monolayers of hexagonal bn,” Phys. Rev. B 66, 235415 (2002). 8 J. X. Cao, X. H. Yan, Y. Xiao, Y. Tang, and J. W. Ding, “Exact study of lattice dynamics of single-walled carbon nanotubes,” Phys. Rev. B 67, 045413 (2003). 9 E. Dobardzic, I. Milosevic, B. Nikolic, T. Vukovic, and M. Damnjanovic, “Single-wall carbon nanotubes phonon spectra: Symmetry-based calculations,” Phys. Rev. B 68, 045408 (2003). 10 D. Sanchez-Portal, E. Artacho, J. M. Soler, A. Rubio, and P. Ordejon, “Ab initio structural, elastic, and vibrational properties of carbon nanotubes,” Phys. Rev. B 59, 12678 (1999). 11 V. N. Popov, “Low-temperature speciﬁc heat of nanotube systems,” Phys. Rev. B 66, 153408 (2002). 12 L.-H. Ye, B.-G. Liu, D.-S. Wang, and R. Han, “Ab initio phonon dispersions of single-wall carbon nanotubes,” Phys. Rev. B 69, 235409 (2004). 13 Y. N. Gartstein, “Vibrations of single-wall carbon nanotubes: Lattice models and low-frequency dispersion,” Phys. Lett. A 327, 83–89 (2004). 14 V. N. Popov and P. Lambin, “Radius and chirality dependence of the radial breathing mode and the g-band phonon modes of single-walled carbon nanotubes,” Phys. Rev. B 73, 085407 (2006). 15 V. N. Popov and P. Lambin, “Vibrational and related properties of carbon nanotubes,” in Carbon Nanotubes (Springer, The Netherlands, 2006). 16 J. Zimmermann, P. Pavone, and G. Cuniberti, “Vibrational modes and low-temperature thermal properties of graphene and carbon nanotubes: Minimal force-constant model,” Phys. Rev. B 78, 045410 (2008). 17 H. Tang, B.-S. Wang, and Z.-B. Su, “Graphene simulation,” in Symmetry and Lattice Dynamics (InTech, Shanghai, China, 2011), Chap. 10. 18 V. N. Popov, V. E. V. Doren, and M. Balkanski, “Elastic properties of single-walled carbon nanotubes,” Phys. Rev. B 61, 3078 (2000). 19 G. D. Mahan, “Oscillations of a thin hollow cylinder: Carbon nanotubes,” Phys. Rev. B 65, 235402 (2002). 20 H. Suzuura and T. Ando, “Phonons and electron-phonon scattering in carbon nanotubes,” Phys. Rev. B 65, 235412 (2002). 21 G. D. Mahan and G. S. Jeon, “Flexure modes in carbon nanotubes,” Phys. Rev. B 70, 075405 (2004). 22 T. Dumitrica and R. D. James, “Obejective molecular dynamics,” J. Mech. Phys. Solids 55, 2206–2236 (2007). 23 A. Aghaei, K. Dayal, and R. S. Elliott, “Symmetry-adapted phonon analysis of nanotubes,” J. Mech. Phys. Solids 61, 557–578 (2013). 24 K. Komatsu, “Theory of the speciﬁc heat of graphite,” J. Phys. Soc. Jpn. 6, 438–444 (1951). 25 K. Komatsu, “Theory of the speciﬁc heat of graphite II,” J. Phys. Soc. Jpn. 10, 346–356 (1955). 26 I. M. Lifshitz, “Thermal properties of chain and layered structures at low temperatures,” Zh. Eksp. Teor. Fiz. 22, 475–486 (1952). 27 K. Komatsu, “Particle-size effect of the speciﬁc heat of graphite at low temperatures,” J. Phys. Chem. Solids 6, 380–385 (1958). 28 B. T. Kelly and P. L. Walker, “Theory of thermal expandion of a grphite crystal in the semi-continuum model,” Carbon 8, 211–226 (1970). 29 R. A. Suleimanov and N. A. Abdullaev, “The nature of negative linear expansion of graphite crystals,” Carbon 31, 1011–1013 (1993). 30 H. Zabel, “Phonons in layered compounds,” J. Phys.: Condens. Matter 13, 7679–7690 (2001). 31 € G. Savini, Y. J. Dappe, S. Oberg, J.-C. Charlier, M. I. Katsnelson, and A. Fasolino, “Bending modes, elastic constants and mechanical stability of graphitic systems,” Carbon 49, 62–69 (2011). 32 E. B. Tadmor and R. E. Miller, Modeling Materials: Continuum, Atomistic and Multiscale Techniques, 1st ed. (Cambridge University Press, 2011). 33 A. Aghaei and K. Dayal, “Symmetry-adapted non-equilibrium molecular dynamics of chiral carbon nanotubes under tensile loading,” J. Appl. Phys. 109(12), 123501 (2011). Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 023503-7 34 Aghaei, Dayal, and Elliott A. Aghaei and K. Dayal, “Tension-and-twist of chiral nanotubes: Torsional buckling, mechanical response, and indicators of failure,” Modell. Simul. Mater. Sci. Eng. 20, 085001 (2012). 35 J. Tersoff, “Empirical interatomic potential for carbon, with applications to amorphous carbon,” Phys. Rev. Lett. 61(25), 2879–2882 (1988). 36 N. Nishiguchi, Y. Ando, and M. N. Wybourne, “Acoustic phonon modes of rectangular quantum wires,” J. Phys.: Condens. Matter 9, 5751 (1997). J. Appl. Phys. 113, 023503 (2013) 37 The conclusions of this study appear mixed. In the authors’ words: “We have shown that ﬂexure modes, those with x / q2 at long wave length, exist in carbon nanotubes. We also ﬁnd that the ﬂexure modes cross over to linear dispersion at very small values of wave vector. We are unsure whether this cross over is a feature of our choice of spring constants, or is an actual feature of nanotubes.” 38 Note, these equations correspond to the results of Lifshitz’s work. Komatsu gives similar expressions except that he replaces the coefﬁcients of the wave vector components by the squared sound velocities of graphite. Downloaded 10 Jan 2013 to 128.2.73.70. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions